OPEN

received: 30 October 2015 accepted: 11 August 2016 Published: 07 September 2016

Newtype single-layer magnetic semiconductor in transition-metal dichalcogenides VX2 (X = S, Se and Te) Huei-Ru Fuh1, Ching-Ray Chang1, Yin-Kuo Wang2, Richard F. L. Evans3, Roy W. Chantrell3 & Horng-Tay Jeng4,5 We present a newtype 2-dimensional (2D) magnetic semiconductor based on transition-metal dichalcogenides VX2 (X = S, Se and Te) via first-principles calculations. The obtained indirect band gaps of monolayer VS2, VSe2, and VTe2 given from the generalized gradient approximation (GGA) are respectively 0.05, 0.22, and 0.20 eV, all with integer magnetic moments of 1.0 μB. The GGA plus on-site Coulomb interaction U (GGA + U) enhances the exchange splittings and raises the energy gap up to 0.38~0.65 eV. By adopting the GW approximation, we obtain converged G0W0 gaps of 1.3, 1.2, and 0.7 eV for VS2, VSe2, and VTe2 monolayers, respectively. They agree very well with our calculated HSE gaps of 1.1, 1.2, and 0.6 eV, respectively. The gap sizes as well as the metal-insulator transitions are tunable by applying the in-plane strain and/or changing the number of stacking layers. The Monte Carlo simulations illustrate very high Curie-temperatures of 292, 472, and 553 K for VS2, VSe2, and VTe2 monolayers, respectively. They are nearly or well beyond the room temperature. Combining the semiconducting energy gap, the 100% spin polarized valence and conduction bands, the room temperature TC, and the in-plane magnetic anisotropy together in a single layer VX2, this newtype 2D magnetic semiconductor shows great potential in future spintronics. The semiconductor-based spintronics has attracted worldwide attention in recent years because of the allowable spin current transport without the presence of a net charge current, which could avoid problems arising from capacitances and Joule heating1. For example, the spin pumping2 or the spin Seebeck effect3,4 have successfully created pure spin currents by using the thermal gradients across a ferromagnetic layer. In many cases, it involves Y5Fe3O12 (YIG) as the magnetic insulator and Pt as the spin current detector5,6, in which the spin current is transformed into an observable transverse voltage by the inverse spin Hall effect7,8. A new type of magnetoresistance (MR) in a Pt-YIG hybrid structure has been discovered5,9 and used in transforming magnetic data and memory storage10–14. The next generation spintronic devices can base on room temperature ferromagnetic semiconductors or heterostructures combining ferromagnetic metals with non-magnetic semiconductors. Nevertheless searching for semiconducting materials with strong ferromagnetism and higher TC is extremely difficult due to the conflicting requirements in the crystal and electronic structures of semiconductors and ferromagnets12. To date all the discovered ferromagnetic semiconductors exhibit magnetic order below room temperature, e.g., EuO (TC = 77 K15), BiMnO3 (TC = 100 K16), La2NiMnO6 (TC = 280 K17), and diluted magnetic semiconductor (DMS) such as the prototypical system (Ga, Mn)As and the newly reported (Ba1−xKx)(Zn1−yMny)2As2 (TC = 185 K, 180 K18). The only exception is the ferrimagnetic insulator Y3Fe5O12 (YIG) with a very high TC = 550 K19 far beyond room temperature. This is the reason why most of the spintronics related works rely on YIG. Meanwhile all of the know magnetic semiconductors belong to 3-dimensional bulk materials.

1

Graduate Institute of Applied Physics, National Taiwan University, Taipei 106, Taiwan. 2Center for General Education and Department of Physics, National Taiwan Normal University, Taipei 106, Taiwan. 3Physics Department, The University of York, York, YO10 5DD, UK. 4Department of Physics, National Tsing Hua University, Hsinchu 30013, Taiwan. 5Institute of Physics, Academia Sinica, Taipei 11529, Taiwan. Correspondence and requests for materials should be addressed to H.-T.J. (email: [email protected]) Scientific Reports | 6:32625 | DOI: 10.1038/srep32625

1

www.nature.com/scientificreports/ Two-dimensional materials such as graphene, boron nitride, and transition metal dichalcogenides (TMDs)20–22 with the single-layer thickness less than 1 nm have attracted tremendous attention in recent years. Because of the more than 40 different families23–26 and the rich electronic properties that can create extensive applications, the TMD has become a rapidly growing research field in the past few years. Representative TMDs such as MoS2, MoSe2, WS2, and WSe2 in the monolayer (ML) form are identified as direct-band-gap semiconductors. With the time reversal symmetry preserved, giant spin splittings of 148–456 meV resulting from missing inversion symmetry and existing spin-orbit coupling20,27,28 could be of high potential in spintronics. However, it is still a challenge to coordinate the TMDs into nanoelectronics29,30. Therefore, developing a new type 2D TMD with exotic electronic properties is imperative. Very recently, a new 2D TMD, few layer Vanadium disulfide (VS2), has been synthesized experimentally31,32. The intrinsic ferromagnetism and potential applications attract particular interests31,33,34. The magnetic moments and magnetic coupling strength of the ultrathin VS2 nanosheets could be tuned by the isotropic strain34. The ferromagnetism provides a new opportunity to fabricate ferromagnetic 2D TMDs without introducing magnetic transition metal atoms or tensile strains34. The synthesis procedures are flexible for other VX2 such as VSe2 and VTe2 monolayers. Besides the bulk VX225, recent phonon dispersion calculations also reveal that monolayer VX2 are stable24. In this work, we systematically investigate the electronic structures of monolayer and multilayer VX2 (X = S, Se and Te) in the 2H-phase based on the generalized gradient approximation (GGA) within the density function theory (DFT). We demonstrate that H-VX2 monolayers exhibit indirect semiconducting energy gaps with intrinsic ferromagnetism and in-plane magnetic anisotropy, achieving an exceptional 2-D magnetic semiconductor group. The magnitude of the band gap and even the metal-insulator transition (MIT) are tunable by applying the in-plane strain and/or changing the number of stacking layers. The GGA plus on-site Coulomb interaction (GGA + U) scheme, the GW approximation, as well as the HSE functional have been adopted to account for the strong correlation effect in transition-metal ions and for the well-known underestimation of the semiconducting band gaps. The Curie temperatures (TC) estimated by Monte Carlo simulations are close to or well beyond the room temperature, which makes this TMD family of high potential in real applications.

Computational Details

The electronic structure calculations of bulk and monolayer VX2 are performed using the projector augmented wave (PAW) method with the Perdew-Burke-Ernzerhof (PBE) generalized gradient approximation (GGA)35 as implemented in the VASP package36,37. The energy cutoff of 400 eV is used for the plane-wave basis expansion with the total energy convergence criteria of 1 × 10−5 eV per unit cell. Gamma-centered k-grids 16 × 16 × 1 were sampled over the 2D Brillouin Zone. Optimized monolayer structures are obtained with the residual force and stress less than 0.01 eV/Å and 1.0 kBar, respectively. For few layered 2H-VX2 calculations, the van der Waals corrections (vdW-DF)38 are adopted to optimized the lattice structural parameters and bondlengths. With vdW correction, the intra-layer bond lengths are hardly changed, while the inter-layer bondlengths are significantly reduced, confirming that the interactions between VX2 layers of weak and non-local vdW type force. The on-site Coulomb energy U = 2 eV and J = 0.87 eV for V 3d electrons39 are taken into account for the electron-electron correlation effects of the localized V-3d orbitals in the GGA + U40 calculations. To correct the underestimated semiconducting band gaps, the GW formalism within a many-body quasiparticle framework is utilized to amend errors in the one-electron Kohn-Sham eigenvalues41,42. The Green’s function G0 and the screened potential W0 in the GW approach (G0W0) based on GGA and GGA + U ground states43 is adopted and henceforth denoted by GW for simplicity. The number of conduction bands nc,max = 591 is sufficient to clearly resolve the peak structure of the imaginary part of the dielectric function. Similar to refs 44 and 45, the convergences of G0W0 energy gaps of VX2 monolayers upon the k-point mesh and the vacuum thickness have been carefully examined with the k-point mesh ranging from 12 × 12 × 1 to 30 × 30 × 1 and the vacuum thickness ranging from 15 Å up to 70 Å and then extrapolated to the infinite vacuum thickness limit. To go beyond the standard GGA approach, calculations based on the HSE46 functional have also been performed for comparison with the converged G0W0 energy gaps.

Results and Discussion

VX2 monolayer structure. The bulk VX2 (X = S, Se, and Te) can be formed in two common TMD structures: 2H (D3h) and 1T (D3d) polymorphs25,31,33. The 2H-TMDs contain two hexagonal monolayers in the unit cell with an AbA stacking sequence in each layer that the V ion is sandwiched by two X ions as shown in Fig. 1. The 1T unit cell consists of only one trigonal monolayer with an AbC stacking sequence in the monolayer. The bulk and multilayer VS2 in the 2H and 1T structures have been synthesized in recently years33,47–50. However, the bulk VSe2 and VTe2 and multilayer VSe2 can only be synthesized in the 1T structure to date51–54. The 1T-VX2 (X = S, Se, and Te) monolayer series is metallic with higher formation energies than the 2H-VX233, therefore they are not considered in this work. Figure 1 shows the 1H lattice structure of the monolayer VX2. Each V ion is surrounded by six neighboring X ions, while each X ion has three neighboring V ions. The V ions occupy the center of a trigonal prism spanned by the X ions (point group P6M2 (D3h)). The structural parameters of monolayer VX2 are determined by the geometry optimization as shown in Table 1. The calculated lattice constant of VS2 and VSe2 are 3.173 and 3.325 Å, respectively, being in excellent agreement with previously calculated results34. The V-X bondlength, the interlayer distance between the two X layers and between the V and X layers also agree well with previous studies34. The geometrically optimized VTe2 monolayer has the largest structural parameters because of the larger atomic radius among the three materials. Ferromagnetism and magnetic anisotropy. The spin-polarized band structures of monolayer VX2 along the high symmetry lines are shown in Fig. 2. The upper and lower panels show GGA and GGA + U results,

Scientific Reports | 6:32625 | DOI: 10.1038/srep32625

2

www.nature.com/scientificreports/

Figure 1. The 1H lattice → structure of the monolayer VX2 (X = S, Se, and Te). (a,b) are the top and side views, a and b are the primitive lattice vectors of the 2D hexagonal unit cell. respectively. → (Å)

a

a(Theo.)

dV−X

dX−X

ΔV−X

VS2

3.173

3.17434

2.362

2.982

1.491

VSe2

3.325

3.33134

2.501

3.205

1.602

VTe2

3.587

–

2.715

3.510

1.755

Table 1. Optimized lattice constant a, V-X bondlength dV−X, interlayer distance between two X layers dX−X and between V and X layers ΔV−X of monolayer VX2 (X = S, Se, and Te). respectively. The GGA calculations show spin polarized bands around the Fermi level (EF) with indirect band gaps of 0.05~0.22 eV originated from the exchange splitting of the V-dz2 bands, and integer magnetic moments of 1.0 μB/f.u. for all the three cases. These results lead to the desirable 2D ferromagnetic semiconducting ground state. To examine the possible antiferromagnetism (AFM), we have adopted the 2 × 2 × 1 supercell for the stripe type AFM arrangement. The calculated total energies demonstrate the ferromagnetic (FM) ground state for all the three VX2 monolayers, being consistent with previous studies34,55,56. The Stoner criterion has been successfully applied to predict the magnetism of different compounds57. If the Stoner criterion58 ID(EF) ≥ 1 is satisfied, then the compound is ferromagnetic in nature at T = 0, where D(EF) is the density of states (DOS) at EF and I is the Stoner parameter measuring the strength of the exchange correlation. Here we adopt this criterion to examine the observed magnetism of VX2. Given from previous first principles calculations, the Stoner parameter I for the V atom is 0.859. Non-magnetic calculations show large D(EF) values of 3.7, 4.4, 5.4 states per eV per atom for VS2, VSe2, and VTe2, respectively. The high DOS at the Fermi level thus cause the Stoner instability, leading to the exchange splits and the intrinsic 2D ferromagnetic ordering. The atom and orbital decomposed band structures of VX2 monolayers from GGA calculations with the spin-orbit coupling (SOC) included self-consistently are shown in Fig. 3. Due to the weak SOC in 3d element V, the overall band structures are more or less the same as the non-spin-orbit counterparts shown in Fig. 2. The atom-decomposed band structures in the upper panels show that the V ion predominates the top most spin up valence band and the lowest spin down conduction band around the EF, while the X ion contributes only slightly to these bands, indicating the 2D ferromagnetism originates mainly from the V ions rather than from the X ions. The d-orbital-decomposed band structures of V ions are depicted in the middle panels of Fig. 3. For VS2 monolayer, the V-d z 2 orbital predominates the valence band maximum (VBM) at Γ and the conduction band minimum (CBM) around M are mainly the d z 2 and dxy hybridized states. While for VSe2, the V-d x 2−y 2 electrons dominate the VBM at K and the CBM around M are mainly the d z 2 and dxy mixed states. As for the VTe2 case, the Scientific Reports | 6:32625 | DOI: 10.1038/srep32625

3

www.nature.com/scientificreports/ 2.5 2 1.5

Energy (eV)

1 0.5

GGA

0

GW

-0.5 -1

(a)

(c)

(b)

2.5 2

Energy (eV)

1.5 1

VS2

0.5 0 -0.5 -1

HSE M

Γ

(d)

VTe2

VSe2

GGA+U

K M

Γ

(e)

K

M

Γ

(f)

K

Figure 2. Spin-polarized band structures of VX2 monolayers without (upper panels) and with (lower panels) the on-site Coulomb energy (GGA + U) U = 2.0 eV and J = 0.87 eV for V 3d orbitals. The blue and red lines denote the spin up and down channels, respectively. The EF (dotted horizontal line) is set at 0 eV. The GW/HSE highest valence and lowest conduction bands are denoted by green/purple star symbols in the upper/ lower panels.

VBM at Γ is replaced by the V-dyz and dxz hybridized bands arising from lower energies with the CBM around M being the d z 2 and dxy hybridized states. The bottom panels of Fig. 3 illustrate the orbital contributions from the X ions. All the S, Se and Te ions play insignificant roles in the bands near the Fermi level. The above results demonstrate that these ~100% spin polarized bands around EF in VX2 monolayer stem mainly from the the V-3d local moments, being consistent with previous reports32. This new 2D ferromagnetic semiconducting material not only provides controllable spin current applications but also regards the spin filter devices by tuning the Fermi level appropriately. Note that the band structures of VX2 are unlike the MoS2 ones. In the latter case, giant spin splittings of 148–456 meV, resulting from the stronger spin-orbit coupling in 4d orbitals and the missing inversion symmetry26, can be found around the K-points with spin bands degenerate elsewhere, reserving the global time reversal symmetry in MoS2. Table 2 shows the calculated magnetocrystalline anisotropy energies (MAE) of the VX2 monolayers in the optimized structures. MAE, the total energy difference between two magnetization directions, serves as a measure of the magnetic easy-axis of a material. The total energy calculations are performed with the spin-orbit coupling included self-consistently over the 20 × 20 × 1 k-mesh in the 2D Brillouin Zone under the energy convergence criteria of 10−8 eV. The out-of-plane MAE is the energy difference between the perpendicular [001] and parallel [100] magnetization directions defined as E[100]-E[001]. While the in-plane MAE, defined as E[100]-E[010], is the energy difference between two in-plane magnetization directions [100] and [010]. The out-of-plane MAE of VS2, VSe2, and VTe2 are −0.21, −0.60, and −1.78 meV/f.u., respectively. These negative out-of-plane MAEs indicate the in-plane magnetic anisotropy (in-plane easy axis of magnetization) for all the three VX2 monolayers, yielding the BKT magnetic transition in the 2D XY model for future spintronic applications. As for the in-plane MAEs, the calculated E[100]-E[010] values are 2 order of magnitude smaller and play insignificant roles only.

Band gap properties. The calculated energy gaps from GGA, GGA + SO, GGA + U, GGA + U + SO (U = 2, J = 0.87 eV), GW, as well as HSE for geometrically optimized VX2 (X = S, Se, and Te) monolayers are all listed in Table 3 for a systematical comparison. In the GGA scheme, the calculated indirect band gaps are 0.046, 0.225, and 0.201 eV for VS2, VSe2, and VTe2 MLs, respectively. As shown in Fig. 2, the CBM of VS2 is close to the M-point along the Γ-M direction and the VBM is located at the Γ-point. The overall band dispersion of VSe2 is similar to Scientific Reports | 6:32625 | DOI: 10.1038/srep32625

4

www.nature.com/scientificreports/

Figure 3. Atom and orbital decomposed band structures of VS2 (left hand side panels), VSe2 (middle panels), and VTe2 (right hand side panels) from GGA with spin-orbit coupling (SOC) included selfconsistently. The upper panels are the atom-decomposed band structures with the green and blue colors denote the components from V and X ions, respectively. The middle panels and bottom panels are the orbital decomposed band structures for V and X ions, respectively. The colors represent the contributions from different orbitals as indicated in the figures.

VS2

VSe2

VTe2

E[100]-E[001] (meV)

−0.21

−0.60

−1.78

E[100]-E[010] (μeV)

−3

−7

−8

Table 2. Calculated magnetic anisotropy energies of the VX2 monolayers. the VS2 one. The only difference is that the VBM goes to the K-point. The band structures of VTe2 are different from the previous ones in two aspects: Firstly, the VBM moves back to the Γ-point due to the rising dxz-dyz hybridized band from lower energies (Fig. 3). Secondly, this emergent top valence band is of the same spin as the bottom conduction band, resulting in the band gap between the same spin polarized bands (Fig. 2). This is very different from the energy gaps between opposite spin channels in VS2 and VSe2 (Fig. 2). To examine the importance of the spin-orbit interaction on the exchange splitting gaps, we have done calculations with the spin-orbit coupling (SOC) included self-consistently. As expected for 3d transition-metal ions that Scientific Reports | 6:32625 | DOI: 10.1038/srep32625

5

www.nature.com/scientificreports/ (eV)

GGA

GGA + SO

GGA + U

GGA + U + SO

GW

HSE

VS2

0.046

0.044

0.473

0.473

1.334

1.110

VSe2

0.225

0.251

0.651

0.684

1.200

1.150

VTe2

0.201

0.149

0.379

0.282

0.705

0.560

Table 3. Calculated energy gaps from GGA, GGA + SO, GGA + U, GGA + U + SO with U = 2, J = 0.87 eV, GW, and HSE for geometrically optimized VX2 (X = S, Se, and Te) monolayers. 0.4 0.3

Energy gap (eV)

0.2 0.1 0 -0.1

VS2

-0.2

VTe2

-0.3

VSe2

-4

-2

0

2 4 strain (%)

6

8

10

Figure 4. The GGA energy gap of the VX2 monolayer as a function of the strain.

the weak SOC plays insignificant roles, the overall electronic and magnetic properties remain more or less the same. The only noticeable change is in the VTe2 band structures (Fig. 3), in which the degeneracy of the highest valence bands at Γ is lifted and the band energy at K is lowered by the SOC, as compared with the non-spin-orbit counterparts in Fig. 2. The enhanced SOC effect in these V-3d bands is induced by Te with stronger SOC in its 5p orbitals. Hence the energy gaps of VS2, VSe2, and VTe2 change slightly to 0.044, 0.251, and 0.149 eV, respectively, as shown in Table 3. To take into consideration the strong electron correlations in the relatively localized 3d orbitals, we perform GGA + U band structure calculations as shown in the lower panels of Fig. 2. The on-site Coulomb repulsion U of 2 eV enhances the exchange splitting and gives rise to larger energy gaps of 0.473, 0.651, and 0.379 eV for VS2, VSe2, and VTe2, respectively, as listed in Table 3. Besides the significantly raised exchange gaps, the CBM and VBM locations of VS2 and VSe2 remain the same as those from GGA. However for the VTe2 case, the CBM from GGA + U locates at the K-point rather than around the M-point given by GGA. Finally the combined SOC and on-site Coulomb repulsion U effect slightly changes the GGA + U energy gaps as listed in Table 3. The broadest energy gap obtained from standard DFT (GGA and GGA + U) calculations is 0.684 eV of VSe2, which is adequately large for real applications. As mentioned above, the on-site Coulomb repulsion U of 2 eV used in this work is given from a previous theoretical estimation for V atoms39. Since the U value of the same element in different materials also depends on the ionicity and the composition of the embedded compound, the precise value of U in VX2 is actually unknown. Because of the uncertainty of the U value, we therefore consider the GW correction which would give the most reliable band gaps in semiconducting materials. To compare with the standard GGA band structures, the GW approximation corrected band energies with carefully examined convergence upon vacuum thickness and number of k-points are denoted by green star symbols in the upper panels of Fig. 2. For simplicity we only depict the highest valence states and lowest conduction states with the top most GW valence band energies aligned at Ef. The GW corrected VBM and CBM of VS2 are located at Γ- and M-point, respectively. While for VSe2 and VTe2, the VBM and CBM are located at K- and M-point, respectively. The GW corrected band gaps are raised to 1.334, 1.200, and 0.705 eV for VS2, VSe2, and VTe2 monolayers, respectively, as shown in Table 3. To go beyond the standard GGA and GGA + U approach, we also adopt the HSE functional to calculate the band structures of VX2 monolayers as denoted by purple star symbols in the lower panels of Fig. 2 (only bands closest to Ef are depicted). The resultant HSE energy gaps of 1.110 eV, 1.150 eV, and 0.560 eV for VS2, VSe2, and VTe2 monolayers, respectively, are also listed in Table 3. As can be seen, the HSE energy gaps agree very well with the converged G0W0 results at the infinite vacuum thickness limit. The GGA energy gap of VX2 monolayer as a function of the strain from −4% up to 10% is shown in Fig. 4. For VS2, the energy gap remains more or less the same below 6% strain, and then turns into the gapless metallic state. While for the other two cases, the energy gap increases below 4% and then decreases to a negative value (corresponding to the band overlap value) above 8% strain. In all cases the tensile strain affects the gap size significantly and eventually induces the metal-insulator transition (MIT) as shown in Fig. 4. This is because that the unoccupied dz2 band at the K-point shifts downward below the EF at high tensile strains due to the reduced Coulomb repulsion, and finally closes the energy gaps of the VX2 monolayers. We note that VTe2(VSe2) Scientific Reports | 6:32625 | DOI: 10.1038/srep32625

6

www.nature.com/scientificreports/ 1.4

VTe2 HSE VSe2 HSE VS2 HSE VTe2 G0W0 VSe2 G0W0 VS2 G0W0 VTe2 U(2.0) VSe2 U(2.0) VS2 U(2.0) VTe2 VSe2 VS2

1.2 1 0.8 0.6

Energy gap (eV)

0.4 0.2 0 -0.2 -0.4 -0.6 -0.8

bulk

4 3

1

2 number of layers

Figure 5. The energy gap of VX2 from GGA, GGA + U, GW, and HSE as a function of the number of layers. reaches the maximum energy gap of 0.36(0.28) eV under 2(4)% tensile strain. This strain-induced exchange gap enhancement implies a higher Curie temperature than the strain free one. On the other hand, due to the increased Coulomb repulsions and enhanced band dispersions of these dz2 bands under compressive strains, the energy gaps are therefore suppressed and achieve another MIT under negative strains around −2%, as can be seen in Fig. 4. So far we have demonstrated various effects on the energy gaps of the VX2 monolayers. Below we discuss the dependence of the energy gaps on the thickness of VX2 multilayers. The gap values given from GGA, GGA + U, GW, as well as HSE calculations are summarized in Fig. 5. First of all we would like to emphasize that all kinds of calculations performed in this work demonstrate an exchange splitting energy gap for all the three VX2 monolayers, strongly supporting that the VX2 families in the monolayer form are indeed 2D ferromagnetic semiconductors. While increasing the number of layers would enhance the interlayer interactions and band dispersions, and hence significantly suppress the energy gap. For the bilayer systems, all the GGA gaps are closed while the GGA + U still gives gaps of ~0.23 eV for VSe2 and VTe2. As for the trilayer and thicker systems, the GGA + U gap size decreases further. At the bulk limit, only VSe2 exhibits a gap of about 0.1 eV from GGA + U, while no energy gap can be found for VS2 and VTe2. In comparison with the consistent semiconducting ground state for VX2 monolayers and the diverse results for bilayer and thicker layers, one may conclude that the ferromagnetic semiconducting phase exists only in the monolayer VX2 systems. Any thicker VX2 multilayers would cause the instability of the ferromagnetic semiconducting phase and result in the metallic phase, giving rise to the metal-insulator transition (MIT) upon layer thicknesses. Note that the experimental synthesis of monolayer VX2 is not yet reported, while multilayer VX2 has been demonstrated as a ferromagnetic metal experimentally32.

Exchange interaction parameters and Curie temperature. To find the magnetic ground state of the VX2 monolayers, we considered three possible magnetic configurations within the 2 × 2 × 1 supercell including the ferromagnetic (FM), antiferromagnetic (AFM), and collinear antiferromagnetic (COL) spin arrangements as depicted in the upper panels of Fig. 6. The corresponding total energies of the three cases provide the estimation of the exchange interaction parameters between the nearest-neighbor (NN) couplings J1 and the next-NN (NNN) couplings J2 60,61 as illustrated in the lower panels of Fig. 6. To evaluate the exchange coupling, we consider the calculated total energy of the VX2 monolayer based on GGA-PBE functional as the sum of the NN spin-spin interactions in terms of the spin Heisenberg model, H = E 0 − J 1 ∑ Si ⋅ S j − J 2 < ij >

∑ Si ⋅ S j ,

ij

(1)

where and ≪ij≫ are respectively the summation over the NN and NNN V site i and site j, and Si (Sj) is the unit vector representing the direction of the local magnetic moment at site i(j). J > 0 is assumed for the FM interaction, and J